FSC 9310 JCP E30
OFFSET MAP, LITHOGRAPHIC–FINISH
Map Paper February 1, 1999
Use information: This paragraph is informational only and is not exclusively definitive of the end use.
For high quality multicolor offset printing of maps, folded inserts, etc. Printed matter may include text, line illustrations, and
halftones up to 150-line screen.
Stock: 100 pct bleached chemical woodpulp. The use of melamine- Water resistance: Average
formaldehyde or any material that releases formaldehyde into not less than (seconds) ........ 20 25 30 35
the atmosphere at concentration of 0.1 ppm or greater shall not Smoothness: Average, each
be permitted in the manufacture of this paper. 140
side (units) ........................... 140 140 140
Note: 1 Not less than 30 pct postconsumer fiber. Any percent to 80 to 80 to 80 to 80
over 30 percentage points, is encouraged, provided that the re- Writing quality: Characters written with ball point and felt tip
quirements of this Standard are met. pens shall be clear cut and free from excessive feathering.
Acidity: pH value shall average not less than 4.8.
Erasing quality: Paper shall retain good ruling, writing, and typ-
Grammage (g/m2) ....................... 60 75 90 105 ing quality, texture, and surface appearance, without ink
Basis weight: 25 by 38 inches, spreading after repeated erasures. After erasures and burnish-
500 sheets (pounds) ................. 40 50 60 70 ing, texture shall permit redrawing of sharp lines in ink.
A tolerance of ±5 pct shall be allowed. Blocking: Sheets shall not stick together after being wet with
Folding endurance: M.I.T., water and then allowed to dry in contact with other sheets of
average, each direction, not the same paper.
less than (double folds) ............ 30 30 35 40
General appearance: Paper shall conform to the standard sam-
Tearing strength: Average, ple(s) adopted by the Government.
each direction, not less than
(mN) .......................................... 290 390 490 580 Color: The paper in the order (or publication) shall be uniform
Equivalent (grams) .................. 30 40 50 60 with a brightness not less than 81 pct. The color variation shall
not exceed DE(CIELAB)=1.0.
Opacity: Average, not less than
(percent) .................................... 88 89 91 92 Formation: Shall be uniform.
No individual specimen shall
average less than (percent) ..... 86 87 89 90 Cleanliness: The dirt count for each side of the paper shall not
exceed 100 specks per square meter. No sample sheet (600 to
Thickness: Average (mm) .......... 0.075 0.090 0.105 0.125 650 cm2 in size) shall contain more than one defect with an
Equivalent (inch) ...................... 0.0030 0.0035 0.0041 0.0049 equivalent area of 0.25 mm2 or greater.
A tolerance of ±0.013 mm (0.0005 inch) shall be allowed.
Paper shall be uniform and shall not vary more than 0.011 mm Sampling and testing: Shall be conducted in accordance with
(0.0004 inch) from one edge to the other. standards in Part 2, Government Paper Specification Standards.
Unless otherwise specified, the following is automatically waived when printing or duplicating is to be accomplished on commercial contract
Equilibrium relative humidity: Shall be 45 pct ±5 pct at 23 ≥C Surface: Shall be free from lint, fuzz, or any particles which will
±2 ≥C. Paper shall be uniform and shall not vary more than 5 pick, lift, fluff, or pile on the blanket under normal press condi-
percentage points in relative humidity from one edge to the tions.
Variations in excess of 5 percentage points shall be sufficient Size and trim: Sheets: Paper shall be furnished in the size(s) or-
cause for rejection of the paper. dered and shall be flat, trimmed square on four sides with clean
smooth edges, and evenly jogged. A tolerance of ±2 mm (1⁄16
Sizing: Paper shall be surface- and internal-sized suitable for sat- inch) shall be allowed except for sheets 216 by 356 mm (81⁄2 by
isfactory printing on both sides of the paper on high-speed offset 14 inches) or less; then a tolerance of ±1 mm (1⁄32 inch) shall be
presses equipped with continuous flow or brush dampening sys- allowed. Successive sheets within any package shall not differ
tems. from each other by more than 0.5 mm (1⁄64 inch). Paper with the
long dimension 813 mm (32 inches) or less shall be considered
Color: Shall match the Government’s standard sample for color. square if the variation does not exceed 1 mm (1⁄32 inch); over
A deviation of DE(CIELAB)±3.0 from the color standard is al- 813 mm (32 inches), 2 mm (1⁄16 inch).
For information only, the CIELAB values (Ill D65, 10° ob- Grain: Direction of the grain on flat paper shall be as ordered.
server) of the color standard are
Mill inspection: Uniformity of color, thickness, and equilibrium
L*=93.5 relative humidity; freedom from foreign matter, either loose or
a*=¥0.5 attached to the paper; and absence of mechanical defects such
b*=1.5 as wrinkles, cuts, slime holes, partial sheets, and dogears; are
Curl: Paper shall lie flat with either no tendency to curl or with all very important. Manufacturers are required to make such in-
a curl which can be overcome under reasonable working condi- spections and tests as will assure freedom from defects in these
1 This requirement may be waived by the ordering agency when purchasing less than a mill run quantity and so stated in the procure-
2 This requirement may be waived in whole or part when so stated in the procurement document. If waived, the following is
Pressroom conditions: The bulk of this paper will be used in air-conditioned pressrooms maintained at 24 °C ±2 °C and 45 pct
±8 pct relative humidity.